### Original Article/Research

## Predicting strength of recycled aggregate concrete using

## Artiﬁcial Neural Network, Adaptive Neuro-Fuzzy Inference System

## and Multiple Linear Regression

### Faezehossadat Khademi

a,⇑### , Sayed Mohammadmehdi Jamal

b### , Neela Deshpande

c### ,

### Shreenivas Londhe

ca_{Department of Civil, Architectural, and Environmental Engineering, Illinois Institute of Technology, Chicago, IL, USA}
b_{Civil Engineering Department, University of Hormozgan, Hormozgan, Iran}

c_{Civil Engineering, Vishwakarma Institute of Information Technology, Pune, India}

Received 26 August 2016; accepted 17 September 2016

Abstract

Compressive strength of concrete, recognized as one of the most signiﬁcant mechanical properties of concrete, is identiﬁed as one of the most essential factors for the quality assurance of concrete. In the current study, three diﬀerent data-driven models, i.e., Artiﬁcial Neural Network (ANN), Adaptive Neuro-Fuzzy Inference System (ANFIS), and Multiple Linear Regression (MLR) were used to pre-dict the 28 days compressive strength of recycled aggregate concrete (RAC). Recycled aggregate is the current need of the hour owing to its environmental pleasant aspect of re-using the wastes due to construction. 14 diﬀerent input parameters, including both dimensional and non-dimensional parameters, were used in this study for predicting the 28 days compressive strength of concrete. The present study concluded that estimation of 28 days compressive strength of recycled aggregate concrete was performed better by ANN and ANFIS in comparison to MLR. In other words, comparing the test step of all the three models, it can be concluded that the MLR model is better to be utilized for preliminary mix design of concrete, and ANN and ANFIS models are suggested to be used in the mix design optimization and in the case of higher accuracy necessities. In addition, the performance of data-driven models with and without the non-dimensional parameters is explored. It was observed that the data-driven models show better accuracy when the non-dimensional parameters were used as additional input parameters. Furthermore, the eﬀect of each non-dimensional parameter on the performance of each data-driven model is investigated. Finally, the eﬀect of number of input parameters on 28 days compressive strength of concrete is examined.

Ó2016 The Gulf Organisation for Research and Development. Production and hosting by Elsevier B.V. All rights reserved.

Keywords: ANN; ANFIS; MLR; Data-driven models; Recycled aggregate concrete

http://dx.doi.org/10.1016/j.ijsbe.2016.09.003

2212-6090/Ó2016 The Gulf Organisation for Research and Development. Production and hosting by Elsevier B.V. All rights reserved.

Abbreviations:ANFIS, Adaptive Neuro-Fuzzy Inference System; ANN, Artiﬁcial Neural Network; MLR, Multiple Linear Regression; NFA, natural ﬁne aggregate; RFA, recycled ﬁne aggregate; NCA10, natural coarse aggregates 10 mm; NCA20, natural coarse aggregates 20 mm; RCA10, recycled coarse aggregates 10 mm; RCA20, recycled coarse aggregates 20 mm; AD, admixture; MSE, mean square value; SSE, sum of squared errors.

⇑ Corresponding author.

E-mail address:faezehossadat_khademi@yahoo.com(F. Khademi).

Peer review under responsibility of The Gulf Organisation for Research and Development. H O S T E D BY

### Gulf Organisation for Research and Development

### International Journal of Sustainable Built Environment

ScienceDirect www.sciencedirect.com

1. Introduction

Scientists have always been concerned about the deplet-ing natural resources and their scarcity has always been one of the most important issues they have been struggling with. Therefore, reducing the impact of this scarcity and protecting the environment has always been an important issue to scientists. One of the achievable keys to decrease this impact may be using construction and demolition waste (C&D) as replacement to natural resources, espe-cially in concrete mix designs. C&D waste, speciﬁcally the concrete waste can be turned to recycled aggregates (RA) which can be used in concrete mixes. Adding the recycled aggregates to concrete mixes is termed as recycled aggre-gate concrete (RAC).

Scientists have investigated the eﬀect of RA on charac-teristics of concrete such as tensile strength, compressive strength, etc. (Ajdukiewicz and Kliszczewicz, 2002; Tu et al., 2006; Deshpande et al., 2011; Ryu, 2002). Using RA as a replacement to natural aggregates would result in the reduction in the compressive strength of RAC since they hold attached mortar to the aggregates. In addition, the pre-vailing criterion for the concrete with RA is the reduction of the density of RAC because of the water absorption by the mortar on the aggregates. Furthermore, the workability of RAC is less than the concrete with conventional aggregates because of the same explained water absorption. Finally, replacing the natural aggregates by RA which would lead to the reduction of the compressive strength might be because of the weaker connections between mortar and RCA (Ajdukiewicz and Kliszczewicz, 2002; Deshpande et al., 2014). Compressive strength of concrete, recognized as one of the most signiﬁcant mechanical properties of con-crete, is identiﬁed as one of the most essential factors for the quality assurance of concrete. Studies have also shown that the level of the compressive strength of RAC highly depends on the strength of RA and therefore, the strength of RAC made of RA with lower strength is less than that of concrete made of RA with higher strength, and the extent of the reduction is dependent on many factors, such as the type of concrete, W/C ratios, moisture percentages, replacement ratios, etc. (Ajdukiewicz and Kliszczewicz, 2002; Tu et al., 2006; Ryu, 2002; Khademi et al., 2015a). Accordingly, this diverse behavior of RA and RAC would lead to widespread testing to reach more understandings of their performances. Nevertheless, these diﬀerent testings are time consuming, expensive, and require large amounts of materials. There-fore, in order to estimate the compressive strength of con-crete, data-driven models which are based on measured data can be a good replacement for this extensive testing.

Scientists have used data-driven models broadly in the ﬁeld of civil engineering. Jiang et al. have found the Artiﬁ-cial Neural Network capable in predicting the concrete cor-rosion of sewers (Jiang et al., 2016).Sadowski and Nikoo (2014) have concluded that the Imperialist Competitive Algorithm is an eﬃcient technique in estimating the corro-sion current density of reinforced concrete (Sadowski and

Nikoo, 2014). Khademi and Behfarnia (2016) have con-cluded that the Artiﬁcial Neural Network is a suitable model in predicting the compressive strength of concrete, however, Multiple Linear Regression is not capable enough in the same prediction purposes (Khademi and Behfarnia, 2016). Nikoo et al. have claimed that the Artiﬁcial Neural Network is a talented method in approximating the dis-placement in concrete reinforcement building (Nikoo et al., 2012). Padmini et al. have successfully used the neuro-fuzzy models in determining the ultimate bearing capacity of shallow foundations (Padmini et al., 2008). (Khademi and Jamal, 2016) have found the Artiﬁcial Neu-ral Network proﬁcient in estimating the 28 days compres-sive strength of concrete (Khademi and Jamal, 2016).

The present study proposes three diﬀerent data-driven models, i.e., Artiﬁcial Neural Network (ANN), Adaptive Neuro Fuzzy Inference System (ANFIS), and Multiple Linear Regression (MLR) models to predict the 28 days compressive strength of concrete using 14 diﬀerent input variables. In addition, the performance of data-driven models with and without the non-dimensional parameters is explored. Furthermore, the eﬀect of each non-dimensional parameter on performance of all the presented data-driven models is investigated. Finally, the eﬀect of number of input parameters on prediction of 28 days com-pressive strength of concrete is studied.

2. Data preparation

In the present study, a total of 257 data sets was col-lected from fresh experiments performed by authors (Ajdukiewicz and Kliszczewicz, 2002; Tu et al., 2006; Ryu, 2002; Deshpande et al., 2014; Hansen and Narud, 1983; Rao et al., 2011; Yong et al., 2009; Akbari et al., 2011; Katz, 2003; Padmini et al., 2002; Dapena et al., 2010; Fathifazl et al., 2009; Agarwal et al., 2011; Yaprak et al., 2011; Schoppe, 2011; Zega and Di Maio, 2009; Duangthidar et al., 2010; Poon et al., 2004; Adnan et al., 2011; Domingo-Cabo et al., 2009; Kou, 2006; Pereira et al., 2012; Lu et al., 2004; Gonc¸alves et al., 2004; Corinaldesi, 2010; Li, 2011). The parameters were divided into three categorizations of mandatory elements, non-dimensional elements, and output elements described in the following:

(A) Mandatory Elements (Raw Data): The weight per cubic meter is considered as raw data based on stan-dard mix design procedures followed worldwide (Deshpande et al., 2014; Sadrmomtazi et al., 2013). In this study, the mandatory parameters are cement (C), natural ﬁne aggregate (NFA), recycled ﬁne aggregate (RFA), natural coarse aggregates 10 mm (NCA10), natural coarse aggregates 20 mm (NCA20), recycled coarse aggregates 10 mm (RCA10), recycled coarse aggregates 20 mm (RCA200), admixture (AD), and water (W).

(B) Non-dimensional Elements: Any ratio of the manda-tory parameters is considered as the non-dimensional elements. In this study, the non-dimensional parame-ters are water-cement ratio (W/C), sand-aggregate ratio (S/A), water to total materials ratio (W/T), replacement ratio of recycled aggregate to natural aggregate by volume (RR), and aggregate to cement ratio (A/C).

(C) Output Element (Dependent Parameter): In this study, the 28 days compressive strength of recycled aggregate concrete is considered as the output parameter.

It is worth mentioning that in this study both the cate-gorization of (A) and (B) are used as input variables and the categorization (C) is used as output variable in the data-driven modeling purposes. The range of these param-eters (Deshpande et al., 2014) is presented inTable 1.

In addition, the number of 28 days compressive strength patterns in each speciﬁc interval is shown inTable 2. 3. Estimation techniques

The prediction models, known as estimators, use the measured data as input variables in their data-driven mod-eling. In all the prediction models, there is a step involved

called ‘‘training step”which assists the model to learn from a collection of training patterns (Khademi and Behfarnia, 2016). In the current study, three diﬀerent data-driven models, i.e. Multiple Linear Regression (MLR), Artiﬁcial Neural Network (ANN), and Adaptive Neuro-Fuzzy Infer-ence System (ANFIS) are used as the prediction models, each explained brieﬂy in the following.

3.1. Multiple Linear Regression model (MLR)

Regression models generally estimate the level of corre-lation between the input and output variables and deter-mine their relationship form. Linear regressions are mostly ﬁtted by the least squares approach, however, they might be ﬁtted using other methods, like by minimizing the ‘‘lack of ﬁt” in some other norms or by minimizing the penalized version of the least squares loss function as in ridge regression. Basically, the linear regression is divided into two categorizations of simple and Multiple Linear Regression. If the aim is to estimate the linear correlation between one predictor and one criterion variable, the model is assumed as the simple linear regression (SLR), however, if the goal is to predict the linear correlation between two or more predictors and still one criterion vari-able, the model is called Multiple Linear Regression (MLR). It is worth mentioning that the MLR is the most common form of linear regression analysis and every value of the independent variable is associated with a value of dependent variable.

Normally, MLR estimates the level of correlation between one response variable (dependent variable) from two or more predictors (Independent variable). It should be emphasized that the MLR explores a correlation in terms of a straight line that best predicts all the individual data points containing both target and output variables (Khademi and Behfarnia, 2016). The general form of a MLR model is as shown in Eq. (1) Chou and Tsai, 2012; Bingo¨l et al., 2013:

Table 1

Characteristics of input and output elements.

Parameter Unit Minimum Maximum

Cement (C) (kg/m3) 235 645

Natural ﬁne aggregate (NFA) (kg/m3) 0 1050

Recycled ﬁne aggregate (RFA) (kg/m3) 0 1050

Natural coarse aggregate 20 mm (NCA20) (kg/m3_{)} _{0} _{1508.64}

Natural coarse aggregate 10 mm (NCA10) (kg/m3_{)} _{0} _{553}

Recycled coarse aggregate 20 mm (RCA20) (kg/m3_{)} _{0} _{1508.64}

Recycled coarse aggregate 10 mm (RCA10) (kg/m3_{)} _{0} _{840}

Water (W) (kg/m3_{)} _{120} _{358}

Admixture (AD) (kg/m3_{)} _{0} _{10.4}

Aggregate to cement ratio (A/C) – 2.279 9.327

Water to cement ratio (W/C) – 0.299 1.028

Sand to aggregate ratio (S/A) – 0.149 1.566

Replacement ratio (RR) (%) – 0 100

Water to total materials (W/T) – 11.287 11.553

28 days compressive strength of concrete (N/mm2) 10.319 100.5

Table 2

Number of patterns in each speciﬁc range of 28 days compressive strength of concrete.

Number Compressive Strength of concrete Range (kg/m3) Number of Patterns 1 0–20 15 2 20–40 110 3 40–60 98 4 60–80 28 5 80–100 5 6 100–150 1 Total 257

^

Y ¼a0þ

Xm j¼1

ajXj ð1Þ

where Yˆ is the model‘s output, X_{j}‘s are the independent
input variables to the model, anda0;a1;a2;. . .;am are

par-tial regression coeﬃcients.

3.2. Artiﬁcial Neural Network (ANN)

Artiﬁcial Neural Network (ANN) is a data processing system inspired by the conﬁguration of the human brain. ANN is basically made of artiﬁcial neurons which are iden-tiﬁed as the highly interconnected processing constituents acting altogether to achieve a speciﬁc problem (Khademi and Jamal, 2016). Generally, ANN is used in complex states where the customary computational techniques are not eﬃcient enough to resolve them.

It is worth mentioning that in the ANN model, the rela-tionship between the predictors and output elements are produced by the data themselves, and accordingly, the ANN is talented to learn from examples widely. In addi-tion, ANN is eﬃcient in incomplete tasks and estimated outcomes. Therefore, these two considerable characteristics distinguish ANN from many other data-driven models and results in usability of high majority of researchers.

The general structure of ANN is shown in Fig. 1. The network contains diﬀerent layers of neurons. In order to predict any measurable functional relation between predic-tors and output parameters to any desirable accuracy, one hidden layer comprising a number of nodes is recom-mended and this recommendation is used in the current study.

The strength of connections is determined using weighted connections. These weights are trained in such as way that assists the ANN model to make the output variables as close as possible to target values. ANN is com-prised of three steps of training, validation, and test. The most important acting of the training step is to minimize

the error function, mean square value (MSE), as n exam-ple, presented in Eq.(2) Chen, 2010; Jang, 1993:

MSE¼_{N}1XN
i¼1

ðtiaiÞ2 ð2Þ

where ‘‘N”is the number of data,tiare the output values, andaiare the target value values.

The validation step which is sometimes called the check step in other data-driven modeling, ANN model, as an example, is used for the construction purposes and per-forms independently from the training step. Lastly, the test step is used to predict the machine algorithm accuracy.

3.3. Adaptive Neuro Fuzzy Inference System (ANFIS)

Adaptive Neuro Fuzzy Inference System (ANFIS) is identiﬁed as a universal estimator for responding to com-plex problems. ANFIS is a class of adaptive, multi-layer and feed-forward networks which is comprised of input– output variables and a fuzzy rule base of the Takagi– Sugeno type. The fuzzy reasoning mechanism of ANFIS model with two fuzzy if-then rules for a ﬁrst-order Sugeno fuzzy model is expressed as (Mosavi and Nik, 2015):

Rule 1: IF x is A1 and y is B1, THEN f1= p1x +

q1y + r1.

Rule 2: IF x is A2 and y is B2, THEN f2= p2 x +

q2y + r2.

The framework of ANFIS contains ﬁve layers, which act diﬀerently from each other; however, the nodes of the same layer perform similar to each other. The structure of ANFIS is shown inFig. 2.

As it is shown inFig. 2, the structure of ANFIS is com-prised of ﬁve diﬀerent layers which are explained brieﬂy in the following:

Layer 1: This layer takes the responsibility for fuzziﬁca-tion of input feature values in the range of 0 to 1. The required values such as membership functions for each ith node are deﬁned in this layer, shown in Eq.(3):

O1

i ¼lAiðxÞ ð3Þ

wherexis the input to nodeiandAiis the linguistic label associated with this node function.

Layer 2: Each rule is a node in the ANFIS by using soft-min or product to ﬁnd out the rule matching factorwi. The incoming signals are multiplied in this layer and sent the product out, shown in Eq.(4).

wi¼lAiðyÞ lBiðyÞ;i¼1;2 ð4Þ

Layer 3: The membership values are getting normalized in this layer. The formulation of normalized ﬁring strength for nodeithin this layer is shown in Eq. (5).

wi¼_{ð}_{w} wi

1þw2Þ;i¼

1;2 ð5Þ

Layer 4: This layer is able to establish the relationship between the input and output values, shown in Eq.(6).

O4

i ¼wiðpixþqiyþriÞ ð6Þ

wherew^_{i}is the output resulted from layer 3, and {p_{i},q_{i},r_{i}}
is the parameter set.

Layer 5: This layer which is also called the de-fuzziﬁcation layer consists of one single node which gener-ates the summation of all incoming signals from previous node and results in a single value. In this layer, each rule output is added to the output layer. Overall output can be calculated using Eq.(7).

O5_{i} ¼X
iwifi¼
P
iwifi
P
iwi
ð7Þ
4. Methodology

In recent years, researchers have investigated widely on various types of civil engineering materials, speciﬁcally concrete and cement (Khademi and Jamal, 2016; Nik et al., 2010; Gandomi et al., 2016; Bahari et al., 2012a; MATLAB and Statistics Toolbox Release, 2014). The 28 days compressive strength of concrete is assumed as the standard compressive strength of concrete, and as a result, in both the engineering decisions and concrete con-structions, estimating the compressive strength of concrete is a signiﬁcant fact (Khademi and Jamal, 2016). In this study, 257 concrete mix designs were used to estimate the 28 days compressive strength of concrete. Three diﬀerent data-driven models, i.e., Multiple Linear Regression (MLR), Artiﬁcial Neural Network (ANN), and Adaptive Neuro-Fuzzy Inference System (ANFIS) were selected as the prediction models and the estimation for the compres-sive strength of concrete has been obtained. The dataset was divided into two subsets of training and testing for the MLR model, however, they were divided into three subsets of training, validation, and testing for both ANN and ANFIS models. All the data driven modeling have been developed in MATLAB software (Nazari and Khalaj, 2012). First, MLR, ANN, and ANFIS models were compared with each other in case of prediction capa-bilities. Next, the sensitivity analysis was performed on the dataset in case of eﬃciency of each single input parameter

on compressive strength of concrete. Finally, the sensitivity analysis was performed in case of the eﬃciency of the num-ber of input parameters on compressive strength of con-crete. The performance criterion for comparing the results is chosen as coeﬃcient of determination (R2), shown in Eq. (8) Nikoo et al., 2015a:

R2_{¼}
P_{n}
i¼1ðyiyÞð^yi^yÞ
2
Pn
i¼1ðyiyÞ
2Pn
i¼1ð^yi^yÞ
2 ð8Þ

where ‘‘y_{i}”is the experimental strength of ‘‘ith” specimen
‘‘y”is the averaged experimental strength, ‘‘^yi”is the

calcu-lated compressive strength of ‘‘i” th specimen, and ‘‘^y” is the averaged calculated compressive strength.

Also, the sum of squared errors (SSE) and Mean squared error (MSE) for all the three models is calculated and compared with each other. The formula of SSE and MSE are presented in Eqs.(9) and (2), respectively: SSE¼XN

i¼1

ðxixiÞ2 ð9Þ

wherenis the number of the specimens,x_{i}is the measured
compressive strength and x_{i} is the predicted compressive
strength.

4.1. Comparison of MLR, ANN, and ANFIS models

In order to compare the MLR, ANN, and ANFIS mod-els, 14 diﬀerent concrete mix parameters have been chosen as input variables. These input parameters are divided into two categorizations of mandatory and non-dimensional elements. Mandatory parameters include cement (C), natu-ral ﬁne aggregate (NFA), recycled ﬁne aggregate (RFA), natural coarse aggregates 10 mm (NCA10), natural coarse aggregates 20 mm (NCA20), recycled coarse aggregates 10 mm (RCA10), recycled coarse aggregates 20 mm (RCA200), admixture (AD), and water (W), and the non-dimensional parameters include water-cement ratio (W/ C), sand-aggregate ratio (S/A), water to total materials ratio (W/T), replacement ratio of recycled aggregate to nat-ural aggregate by volume (RR), and aggregate to cement

ratio (A/C). Following, the performance of each expressed data-driven model in predicting the 28 days compressive strength of concrete is presented.

4.1.1. Multiple Linear Regression model (MLR)

In the MLR model, the data are divided into two subsets of training and test. The proportions of training and testing are characterized based on the fact that the general struc-ture of the model is constructed with respect to the training data set. Therefore, the amount of data in the training set plays a signiﬁcant role. The total number of specimens was equal to 257 in which 85% of them (i.e. 218 specimens) were chosen for the training step, and 15% of them (i.e. 39 spec-imens) were selected for the test step.Fig. 3shows the rela-tionship between the measured and predicted compressive strength of the MLR model for the test step.

As it is shown in the ﬁgure, theR2value of the test step in MLR model is determined as 0.6085. In addition, the SSE and MSE are calculated as 3880.67 and 99.504, respec-tively. To conclude, MLR model did not show the high level of capability in predicting the 28 days compressive strength of concrete. This might be due to the fact that there is nonlinear relationship between the studied param-eters and MLR model is mostly able to ﬁnd out the linear relationship between the response and predictor variables.

4.1.2. Artiﬁcial Neural Network model (ANN)

In the ANN model, the data are divided into three sub-sets of training, validation, and test. The proportions of training, validation, and testing are characterized based on the fact that the general structure of the model is con-structed based on the training data set. The total number of specimens were equal to 257 in which 70% of them (i.e. 179 specimens) were chosen for training step, 15% of them (i.e. 39 specimens) were selected for the validation step, and 15% of them (i.e. 39 specimens) were selected for the test step. In addition, the sigmoidal tangent func-tion was chosen for hidden nodes. Diﬀerent algorithms were tried to ﬁnd the most suitable one, and among all of them, the Levenberg–Marquardt (LM) algorithm was selected. The ANN model was tested only with one hidden layer. Furthermore, in order to approximate the number of hidden nodes in the hidden layer, the experimental formula shown in Eq.(10)was usedSajedi and Huang, 2015a.

NH<¼2N1þ1 ð10Þ

In which NH is the maximum number of nodes in the

hidden layer and N1 is the number of inputs. Therefore,

in this study, based on the number of input variables which was equal to 14, the maximum number of nodes in the hid-den layer was chosen as 29. The structure of the ANN modeling in Matlab environment (Nazari and Khalaj, 2012) with 14 input parameters, 29 hidden nodes in the hid-den layer, and one output parameter [14:29:1:1] is shown in Fig. 4.

Figs. 5 and 6 show the relationship between the mea-sured and predicted compressive strength of the MLR

model for the training and validation steps, respectively.

R2 is a statistical estimation to show how close the mea-sured and predicted values are to each other. As shown in the ﬁgures, in both the training and validation step, the model presents desirable results in case of R values.

In addition, in order to determine the performance of the model, the coeﬃcient of determination (R2) is evaluated for the test step, shown inFig. 7.

As shown in theFig. 7, the coeﬃcient of determination for the testing of the ANN model is determined as

R2= 0.9185. In addition, the SSE and MSE are determined as 770.94 and 19.77, respectively. To conclude, the ANN model is eﬃcient in estimating the compressive strength of concrete, as compared to MLR.

4.1.3. Adaptive Neuro-Fuzzy Inference System (ANFIS)

In this study, the ANFIS modeling was performed in Matlab software and the proportions of training, valida-tion (check), and testing were selected the same as the ones selected for ANN modeling.Fig. 8shows the measured and predicted data for 28 days compressive strength of concrete for the training step.Fig. 8demonstrates good coincidence of target and output data which indicate the capability of the ANFIS model.

In addition,Fig. 9 shows the relationship between the measured and predicted compressive strength for the test-ing of the ANFIS model. The coeﬃcient of determination (R2) shows the level of capability of the ANFIS model in predicting the 28 compressive strength of concrete.

As it is shown in the ﬁgure, the coeﬃcient of determina-tion for the test step of the ANFIS model is determined as

R2= 0.9075. In addition, the SSE and MSE are determined as 992.67 and 25.45, respectively. To conclude, the ANFIS model is found to be capable in estimating the compressive strength of concrete with satisfactory performance.

4.1.4. Comparison of results of MLR, ANN, and ANFIS

In recent years, scientists have performed diﬀerent inves-tigations on various types of civil engineering materials, especially concrete and cement (Sajedi and Huang, 2015b; Khademi et al., 2015b; Bahari et al., 2016, 2012b;

Figure 3. Relationship between the measured and predicted compressive strength of the test step of the MLR model.

Hawkins et al., 2012; Nikoo et al., 2015b; Vu-Bac et al., 2015). The 28 days compressive strength of concrete is assumed as the standard compressive strength of concrete, and therefore, in both the engineering decisions and con-crete constructions, estimating the compressive strength

of concrete is a signiﬁcant fact. In this paper, the perfor-mance of MLR, ANN, and ANFIS on predicting the 28 days compressive strength of concrete based on coeﬃ-cient of determination (R2) and the sum of squared errors (SSE) is studied. The higher values ofR2imply the higher capability of the model in prediction purposes. The values of R2 and SSE for all the three models are shown in Table 3.

As it is illustrated in the Table,R2and SSE values act inversely. ANN model has the higher value ofR2as com-pared to ANFIS and MLR. Therefore, ANN model is found to be the most eﬃcient model in predicting the 28 compressive strength of concrete.

In addition, according to the table, it can be concluded that both the ANN and ANFIS models are capable enough in predicting the 28 days compressive strength of concrete. However, ANN outperforms ANFIS in the same prediction purposes. On the other hand, MLR model is found to be not reliable enough in predicting the 28 days compressive strength of concrete. The higher accuracy of ANN and ANFIS models in comparison to the MLR model may be due to the nonlinear relationship between the parameters which can be presented better by Ann and ANFIS. Nor-mally, the MLR is a suggested model for proposing the pre-liminary mix design, and for higher accuracy necessities, the ANN and ANFIS models are recommended.

4.2. Sensitivity analysis

According to (Vu-Bac et al., 2014) sensitivity analysis (SA) is the investigation of how much model output parameters are inﬂuenced by changes in model input

Figure 4. Structure of ANN model in Matlab environment with 14 input parameters, 29 hidden nodes in the hidden layer, and one output parameter.

Figure 5. Relationship between the measured and predicted compressive strength of the training step of the ANN model.

Figure 6. Relationship between the measured and predicted compressive strength of the validation step of the ANN model.

Figure 7. Relationship between the measured and predicted compressive strength of the test step of the ANN model.

parameters. In this study, the sensitivity analysis is per-formed on the data using ANN and ANFIS models, which were proved capable enough in the prediction purposes in the last section. In this research, the sensitivity analysis is performed from two diﬀerent sides of views; (1) Sensitivity analysis based on eﬃciency of each individual input param-eter on the output value, and (2) Sensitivity analysis based on eﬃciency of number of input parameters on the output value. Both are discussed comprehensively in the following.

4.2.1. Sensitivity analysis based on eﬃciency of each individual input parameter on the output value

In this section, the sensitivity analysis is performed based on the eﬀect of each individual non-dimensional input parameter on the output value. In other words, in order to understand the correlation of each input parame-ter with the output parameparame-ter using ANN and ANFIS models, ANN1, and ANFIS1 were constructed based on the raw data as their input parameters. In addition, in ANN2 and ANIS 2, (S/A) was added as an additional parameter to the already existing ones in ANN1 and ANFIS1. Therefore, the eﬀect of (S/A) on the prediction accuracy of the model was investigated. In the same way, all the other non-dimensional elements i.e. (W/C), (W/T), (A/C), (R/R) were added to ANN1 and ANFIS 1 individ-ually and constructed in a separate network. The details of these ANN and ANFIs models are shown inTable 4.

4.2.1.1. Sensitivity analysis using ANN model. Figs. 10–15 show the relationship between the target and output com-pressive strength of ANN1 to ANN6, respectively, for both the training and validation steps. According to these ﬁg-ures, the performance of ANN1 to ANN6 is shown based on correlation coeﬃcient (R).

Figure 8. Comparison between the ‘‘Target”and ‘‘Output”parameters for ‘‘Training”step in ANFIS model.

Figure 9. Relationship between the measured and predicted compressive strength of the test step of the ANFIS model.

Table 3

R2_{and SSE and MSE values for MLR, ANN, and ANFIS models.}

Data-driven model Coeﬃcient of determination (R2_{)} _{Sum of squared errors (SSE)} _{Mean squared error (MSE)}

MLR 0.6085 3880.67 99.5043

ANN 0.9185 770.94 19.7676

ANFIS 0.9075 992.67 25.4530

Table 4

Characteristics of ANN and ANFIS models based on eﬃciency of each individual input parameter.

Input parameter ANN model ANFIS model

C, NFA, RFA, NC20, NC10, RCA20, RCA10, AD, W ANN1 ANFIS1

C, NFA, RFA, NC20, NC10, RCA20, RCA10, AD, W, A/C ANN2 ANFIS2

C, NFA, RFA, NC20, NC10, RCA20, RCA10, AD, W, S/A ANN3 ANFIS3

C, NFA, RFA, NC20, NC10, RCA20, RCA10, AD, W, W/T ANN4 ANFIS4

C, NFA, RFA, NC20, NC10, RCA20, RCA10, AD, W, R/R ANN5 ANFIS5

In addition, the results of the sensitivity analysis for ANN for test step based on coeﬃcient of determination (R2), the sum of squared errors (SSE), and the mean squared error (MSE) are shown inTable 5.

As it is shown in the table, when SA and RR were added as non-dimensional parameters (ANN3 and ANN5) to the model with just raw data (ANN1), the accuracy of estimat-ing the 28 days compressive strength increases. On the

Figure 10. Relationship between the target and output values for training and validation steps in ANN1.

Figure 11. Relationship between the target and output values for training and validation steps in ANN2.

other hand, adding other non-dimensional parameters like A/C, W/T, and W/C (ANN2, ANN4, ANN6) to the model with raw data (ANN1) has an inverse impact on the

accu-racy of estimating the 28 days compressive strength of con-crete which might be due to the duplication of the information.

Figure 13. Relationship between the target and output values for training and validation steps in ANN4.

Figure 14. Relationship between the target and output values for training and validation steps in ANN5.

Table 5

Values ofR2, SSE, and MSE for Test Step of ANN1 to ANN6.

Model number Coeﬃcient of determination (R2) Sum of squared errors (SSE) Mean squared error (MSE)

ANN1 0.9086 987.1835 25.3124 ANN2 0.9059 1023.276 26.23785 ANN3 0.9132 981.5367 25.16761 ANN4 0.9050 1036.297 26.57172 ANN5 0.9151 959.39 24.59974 ANN6 0.9009 1091.0940 27.97677

Figure 16. Relationship between the measured and predicted compressive strength of the test step of the ANFIS1 model.

Figure 17. Relationship between the measured and predicted compressive strength of the test step of the ANFIS2 model.

Figure 18. Relationship between the measured and predicted compressive strength of the test step of the ANFIS3 model.

Figure 19. Relationship between the measured and predicted compressive strength of the test step of the ANFIS 4 model.

Figure 20. Relationship between the measured and predicted compressive strength of the test step of the ANFIS5 model.

Figure 21. Relationship between the measured and predicted compressive strength of the test step of the ANFIS6 model.

Table 6

Values ofR2, SSE, and MSE for Test Step of ANFIS1 to ANFIS6.

Model number Coeﬃcient of determination (R2) Sum of squared errors (SSE) Mean squared error (MSE)

ANFIS 1 0.9004 1095.052 28.07826 ANFIS 2 0.8996 1109.002 28.43595 ANFIS 3 0.9027 1020.8090 26.17459 ANFIS 4 0.8992 1116.678 28.63277 ANFIS 5 0.9031 1018.63 26.11872 ANFIS 6 0.8987 1130.014 28.97472

Figure 22. Coeﬃcient of Determinations for the test steps of ANN1 to ANN6.

Figure 23. Coeﬃcient of Determinations for the test steps of ANFIS1 to ANFIS6.

Table 7

Characteristics of ANN and ANFIS models based on eﬃciency of number of input parameters on coeﬃcient of determination.

Input parameter ANN model ANFIS model

C, NFA, RFA, NC20, NC10 ANN7 ANFIS7

C, NFA, RFA, NC20, NC10, RCA20 ANN8 ANFIS8

C, NFA, RFA, NC20, NC10, RCA20, RCA10 ANN9 ANFIS9

C, NFA, RFA, NC20, NC10, RCA20, RCA10, AD ANN10 ANFIS10

C, NFA, RFA, NC20, NC10, RCA20, RCA10, AD, W ANN11 ANFIS11

C, NFA, RFA, NC20, NC10, RCA20, RCA10, AD, W, S/A ANN12 ANFIS12

C, NFA, RFA, NC20, NC10, RCA20, RCA10, AD, W, RR ANN13 ANFIS13

Figure 24. Coeﬃcient of determinations for the test steps of ANN7 to ANN13.

Figure 25. Coeﬃcient of determinations for the test steps of ANFIS7 to ANFIS13.

4.2.1.2. Sensitivity analysis using ANFIS model.Figs. 16–21 show the relationship between the target and output com-pressive strength of ANFIS1 to ANFIS6, respectively, for the test step. According to these ﬁgures, the performance of ANFIS1 to ANFIS6 is shown based on coeﬃcient of determination (R2).

In addition, the results of the sensitivity analysis of ANFIS for the test step based on coeﬃcient of determina-tion (R2), the sum of squared errors (SSE), and the mean squared error (MSE) are shown inTable 6.

As it is shown in the table, when the SA and RR were added as non-dimensional parameters (ANFIS3 and ANFIS5) to the model with just raw data (ANFIS1), the accuracy of estimating the 28 days compressive strength increases. On the other hand, adding other non-dimensional parameters like A/C (ANFIS2), W/T (ANFIS4), and W/C (ANFIS6) to the model with raw data (ANFIS1) has an inverse impact on the accuracy of esti-mating the 28 days compressive strength of concrete. This inverse impact on the accuracy of the result might be due to the fact that adding A/C, W/T, and W/C to ANFIs1 would result in the duplication of the information.

4.2.1.3. Results and discussion. Figs. 22 and 23 show the coeﬃcient of determination of constructed ANN and ANFIS models, respectively. It is worth mentioning that all these models are constructed to investigate the eﬃciency of each individual input parameter on the output value.

As it is shown in the ﬁgures, adding SA and RA to the model with just the raw data would lead to increase in the accuracy of predicting the 28 days compressive strength of concrete. However, adding A/C, W/T, and W/C to the model with just the raw data would lead to decrease in the accuracy of estimating the compressive strength of con-crete. This might be due to the fact that adding A/C, W/T, and W/C to raw data would lead to the duplication of information which would result in the reduction of the accuracy of predicting the 28 days compressive strength of concrete.

In addition, comparing all the ANFIS and ANN mod-els, it is illustrated that performance of ANN model is more satisfactory in predicting the 28 days compressive strength of concrete in comparison to ANFIS in terms of coeﬃcient of determination.

4.2.2. Sensitivity analysis based on eﬃciency of number of input parameters on the output value

As it was investigated, adding A/C, W/T, and W/C to the already existing raw data has a negative impact on the coeﬃcient of determination. Therefore, in this part, in order to investigate the eﬀect of the number of input parameters on the coeﬃcient of determination, the raw data and the non-dimensional parameters which had posi-tive impact on the coeﬃcient of determination, i.e., RR and S/A are used as input parameters in this part. Diﬀerent ANN and ANFIS models have been constructed to

inves-tigate the eﬀect of number of input parameters on the coef-ﬁcient of determination, shown in Table 7.

The coeﬃcient of determination (R2) for the test step of all the presented ANN and ANFIS models inTable 7are shown inFigs. 24 and 25, respectively.

As it is shown in the ﬁgures, when the number of input variables increase, the coeﬃcient of determinations increase. In other words, the more the number of input variables are, the more accurate the coeﬃcient of determi-nations would be. It is worth mentioning that all these input variables should be independent from each other to have positive impact on the coeﬃcient of determinations. 5. Conclusion

In this paper, three diﬀerent data driven models, i.e., Artiﬁcial Neural Network (ANN), Adaptive Neuro-Fuzzy Inference System (ANFIS), and Multiple Linear Regression (MLR) were used to predict the 28 days com-pressive strength of recycled aggregate concrete (RAC). The following outcomes have been taken out from this research:

(1) MLR model with R2= 0.6085, SSE = 3880.67, and MSE = 99.5043 was found not to be eﬃcient enough in predicting the 28 days compressive strength of con-crete. This may be because of the nonlinear relation-ship between the studied elements and MLR model is mostly able to ﬁnd out the linear relationship between the input and output variables.

(2) ANN model with R2= 0.9185, SSE = 770.94, and MSE = 19.7676 was found to be capable in estimat-ing the 28 days compressive strength of concrete. (3) ANFIS model with R2= 0.9075, SSE = 992.67, and

MSE = 25.4530 was found to be talented in approxi-mating the 28 days compressive strength of concrete. (4) ANN and ANFIS models were found to be eﬃcient in predicting the 28 days compressive strength of con-crete, however MLR was found not to be capable enough in the same predicting purposes. In other words, MLR model is better to be used for prelimi-nary mix design of concrete, and ANN and ANFIS are recommended in the mix design optimization and in the case of higher accuracy requirements. The advantage of ANN and ANFIS might be due to the fact that the relationship between the studied variables is nonlinear and these two models are more capable in determining the nonlinear relationship between the response and predictor variables. (5) Although both the ANN and ANFIS models are

cap-able enough to estimate the 28 days compressive strength of concrete, ANN was found more eﬃcient than ANFIS.

(6) Adding non-dimensional parameters of SA and RA to the model with just the raw data would lead to increase in the accuracy of predicting the 28 days compressive strength of concrete.

(7) Adding non-dimensional parameters of A/C, W/T, and W/C to the model with just the raw data would lead to decrease in the accuracy of estimating the compressive strength of concrete. This might be due to the fact that adding A/C, W/T, and W/C to raw data would lead to the duplication of information which would result in the reduction of the accuracy of predicting the 28 days compressive strength of concrete.

(8) Increase in the number of independent variables would result in an increase in the accuracy of the model.

References

Adnan, S. H., Abdul Rahman, I., & Mohd Saman, H. (2011). Recycled aggregate as coarse aggregate replacement in concrete mixes. Agarwal, S.D., Karnnkal, A.B., Patil, P.N., 2011. Feasibility study of use

of RCA in concrete. Int. J. Res. Eng. Sci. Technol., 70–75

Ajdukiewicz, A., Kliszczewicz, A., 2002. Inﬂuence of recycled aggregates on mechanical properties of HS/HPC. Cem. Concr. Compos. 24 (2), 269–279.

Akbari, Y.V., Arora, N.K., Vakil, M.D., 2011. Eﬀect on recycled aggregate on concrete properties. Int. J. Earth Sci. Eng. 4 (6), 924–928. Bahari, A., Sadeghi Nik, A., Roodbari, M., Taghavi, K., Mirshaﬁei, S.E., 2012a. Synthesis and strength study of cement mortars containing SiC nano particles. Digest J. Nanomater. Biostructures 7 (4).

Bahari, A., Nik, A.S., Roodbari, M., Mirnia, N., 2012b. Investigation the Al–Fe–Cr–Ti nano composites structures with using XRD and AFM techniques. Sadhana 37 (6), 657–664.

Bahari, A., Berenjian, J., Sadeghi-Nik, A., 2016. Modiﬁcation of Portland Cement with Nano SiC. Proc. Natl. Acad. Sci., India, Sect. A 86 (3), 1– 9.

Bingo¨l, A.F., Tortum, A., Gu¨l, R., 2013. Neural networks analysis of compressive strength of lightweight concrete after high temperatures. Mater. Des. 52, 258–264.

Chen, L., 2010. A multiple linear regression prediction of concrete compressive strength based on physical properties of electric arc furnace oxidizing slag. Int. J. Appl. Sci. Eng. 7 (2), 153–158. Chou, J.S., Tsai, C.F., 2012. Concrete compressive strength analysis using

a combined classiﬁcation and regression technique. Autom. Constr. 24, 52–60.

Corinaldesi, V., 2010. Mechanical and elastic behaviour of concretes made of recycled-concrete coarse aggregates. Constr. Build. Mater. 24 (9), 1616–1620.

Dapena, E., Alaejos, P., Lobet, A., Pe´rez, D., 2010. Eﬀect of recycled sand content on characteristics of mortars and concretes. J. Mater. Civ. Eng. 23 (4), 414–422.

Deshpande, N., Kulkarni, S.S., Patil, N., 2011. Eﬀectiveness of using coarse recycled concrete aggregate in concrete. Int. J. Earth Sci. Eng. 4 (6), 913–919.

Deshpande, N., Londhe, S., Kulkarni, S., 2014. Modeling compressive strength of recycled aggregate concrete by artiﬁcial neural network, model tree and non-linear regression. Int. J. Sustainable Built Environ. 3 (2), 187–198.

Domingo-Cabo, A., La´zaro, C., Lo´pez-Gayarre, F., Serrano-Lo´pez, M. A., Serna, P., Castan˜o-Tabares, J.O., 2009. Creep and shrinkage of recycled aggregate concrete. Constr. Build. Mater. 23 (7), 2545–2553. Duangthidar, K., 2010. Recycled Aggregate Concrete for Structural

Applications (Ph.D. thesis). University of Western Sydney.

Fathifazl, G., Abbas, A., Razaqpur, A.G., Isgor, O.B., Fournier, B., Foo, S., 2009. New mixture proportioning method for concrete made with coarse recycled concrete aggregate. J. Mater. Civ. Eng. 21 (10), 601– 611.

Gandomi, A.H., Sajedi, S., Kiani, B., Huang, Q., 2016. Genetic programming for experimental big data mining: A case study on concrete creep formulation. Autom. Constr. 70, 89–97.

Gonc¸alves, A., Esteves, A., & Vieira, M. (2004). Inﬂuence of recycled concrete aggregates on concrete durability. Proc. RILEM, PRO 40: use of recycled materials in buildings and structures.

Hansen, T.C., Narud, H., 1983. Strength of recycled concrete made from crushed concrete coarse aggregate. Concr. Int. 5 (01), 79–83. Hawkins, D., Hong, S.M., Raslan, R., Mumovic, D., Hanna, S., 2012.

Determinants of energy use in UK higher education buildings using statistical and artiﬁcial neural network methods. Int. J. Sustainable Built Environ. 1 (1), 50–63.

Jang, J.S., 1993. ANFIS: adaptive-network-based fuzzy inference system. IEEE Trans. Systems Man Cybern. 23 (3), 665–685.

Jiang, G., Keller, J., Bond, P.L., Yuan, Z., 2016. Predicting concrete corrosion of sewers using artiﬁcial neural network. Water Res. Katz, A., 2003. Properties of concrete made with recycled aggregate from

partially hydrated old concrete. Cem. Concr. Res. 33 (5), 703–711. Khademi, F., Behfarnia, K., 2016. Evaluation of concrete compressive

strength using artiﬁcial neural network and multiple linear regression models. Iran Univ. Sci. Technol. 6 (3), 423–432.

Khademi, F., Jamal, S.M., 2016. Predicting the 28 days compressive strength of concrete using artiﬁcial neural network. i-Manager’s J. Civ. Eng. 6 (2), 1.

Khademi, F., Akbari, M., Jamal, S.M.M., 2015a. Prediction of compres-sive strength of concrete by data-driven models. i-Manager’s J. Civ. Eng. 5 (2), 16.

Khademi, F., Akbari, M., Jamal, S.M., 2015b. Measuring compressive strength of puzzolan concrete by ultrasonic pulse velocity method. i-Manager’s J. Civ. Eng. 5 (3), 23.

Kou, S., 2006. Reusing Recycled Aggregates in Structural Concrete (Doctoral dissertation). The Hong Kong Polytechnic University. Li, Z., 2011. Advanced Concrete Technology. John Wiley & Sons. Luı’s, R.E., Jorge, C., de Brito, 2004. Criteria for the use of ﬁne recycled

concrete aggregates in concrete production. In: Proceedings of International RILEM Conference on Use of Recycled Building Materials in Building and Structures, Barcelona, Spain, pp. 1–8. MATLAB and Statistics Toolbox Release 2014a, 2014. The Math Works,

Inc, Natick, Massachusetts, United States.

Mosavi, S.M., Nik, A.S., 2015. Strengthening of steel–concrete composite girders using carbon ﬁbre reinforced polymer (CFRP) plates. Sadhana 40 (1), 249–261.

Nazari, A., Khalaj, Gh., 2012. Prediction compressive strength of lightweight geopolymers by ANFIS. Ceram. Int. 38 (6), 4501–4510. Nik, A.S., Bahari, A., Ebadi, A.G., Nik, A.S., Ghasemi-Hamzekolaee, A.,

2010. The role of nano particles (Si) in gate dielectric. Indian J. Sci. Technol. 3 (6), 634–636.

Nikoo, M., Zarfam, P., Nikoo, M., 2012. Determining displacement in concrete reinforcement building with using evolutionary artiﬁcial neural networks. World Appl. Sci. J. 16 (12), 1699–1708.

Nikoo, M., Torabian Moghadam, F., Sadowski,Ł., 2015a. Prediction of concrete compressive strength by evolutionary artiﬁcial neural net-works. Adv. Mater. Sci. Eng. 2015.

Nikoo, M., Zarfam, P., Sayahpour, H., 2015b. Determination of compressive strength of concrete using Self Organization Feature Map (SOFM). Eng. Comput. 31 (1), 113–121.

Padmini, A.K., Ramamurthy, K., Mathews, M.S., 2002. Relative moisture movement through recycled aggregate concrete. Mag. Concr. Res. 54 (5), 377–384.

Padmini, D., Ilamparuthi, K., Sudheer, K.P., 2008. Ultimate bearing capacity prediction of shallow foundations on cohesionless soils using neurofuzzy models. Comput. Geotech. 35 (1), 33–46.

Pereira, P., Evangelista, L., De Brito, J., 2012. The eﬀect of superplas-ticizers on the mechanical performance of concrete made with ﬁne recycled concrete aggregates. Cem. Concr. Compos. 34 (9), 1044–1052. Poon, C.S., Shui, Z.H., Lam, L., Fok, H., Kou, S.C., 2004. Inﬂuence of moisture states of natural and recycled aggregates on the slump and compressive strength of concrete. Cem. Concr. Res. 34 (1), 31–36.

Rao, M.C., Bhattacharyya, S.K., Barai, S.V., 2011. Inﬂuence of ﬁeld recycled coarse aggregate on properties of concrete. Mater. Struct. 44 (1), 205–220.

Ryu, J.S., 2002. An experimental study on the eﬀect of recycled aggregate on concrete properties. Mag. Concr. Res. 54 (1), 7–12.

Sadowski, L., Nikoo, M., 2014. Corrosion current density prediction in reinforced concrete by imperialist competitive algorithm. Neural Comput. Appl., 1627–1638

Sadrmomtazi, A., Sobhani, J., Mirgozar, M.A., 2013. Modeling compres-sive strength of EPS lightweight concrete using regression, neural network and ANFIS. Constr. Build. Mater. 42, 205–216.

Sajedi, S., Huang, Q., 2015a. Probabilistic prediction model for average bond strength at steel–concrete interface considering corrosion eﬀect. Eng. Struct. 99, 120–131.

Sajedi, S., Huang, Q., 2015b. Time-dependent reliability analysis on the ﬂexural behavior of corroded RC beams before and after repairing. Struct. Congr., 1470–1481

Schoppe, B.M., 2011. modulus of elasticity in concrete with recycled aggregates (Doctoral dissertation). California Polytechnic State University, San Luis Obispo.

Tu, T.Y., Chen, Y.Y., Hwang, C.L., 2006. Properties of HPC with recycled aggregates. Cem. Concr. Res. 36 (5), 943–950.

Vu-Bac, N., Lahmer, T., Keitel, H., Zhao, J., Zhuang, X., Rabczuk, T., 2014. Stochastic predictions of bulk properties of amorphous polyethylene based on molecular dynamics simulations. Mech. Mater. 68, 70–84.

Vu-Bac, N., Silani, M., Lahmer, T., Zhuang, X., Rabczuk, T., 2015. A uniﬁed framework for stochastic predictions of mechanical properties of polymeric nanocomposites. Comput. Mater. Sci. 96, 520–535. Yaprak, H., Aruntas, H.Y., Demir, I., Simsek, O., Durmus, G., 2011.

Eﬀects of the ﬁne recycled concrete aggregates on the concrete properties. Int. J. Phys. Sci. 6 (10), 2455–2461.

Yong, P.C., Razali, I., Teo, D.C.L., 2009. Utilisation of recycled aggregate as coarse aggregate in concrete. UNIMAS E J. Civil Eng. 1 (1). Zega, C.J., Di Maio, A.A., 2009. Recycled concrete made with diﬀerent

natural coarse aggregates exposed to high temperature. Constr. Build. Mater. 23 (5), 2047–2052.